| ||Format||Pages||Price|| |
|9||$43.00||  ADD TO CART|
|Hardcopy (shipping and handling)||9||$43.00||  ADD TO CART|
|Standard + Redline PDF Bundle||18||$51.60||  ADD TO CART|
Significance and Use
This test method is not recommended for the acceptance testing of commercial shipments of wool top, card sliver, or scoured wool since the referee method, Test Method D 2130
.If there are differences of practical significance between reported test results for two laboratories (or more), comparative test should be performed to determine if there is a statistical bias between them, using competent statistical assistance. As a minimum, use the samples for such a comparative test that are as homogenous as possible, drawn from the same lot of material as the samples that resulted in disparate results during initial testing and randomly assigned in equal numbers to each laboratory. The test results from the laboratories involved should be compared using a statistical test for unpaired data, a probability level chosen prior to the testing series. If bias is found, either its cause must be found and corrected, or future test results for that material must be adjusted in consideration of the known bias.
The specific area of the wool fibers is measured by the resistance in air flow. The resistance to air flow has been related to average fiber diameter measured by the microprojection method. The instruments have been calibrated to read average diameter in micrometres. Although the reading is affected by the average fiber diameter distribution of the specimen, the results secured by the instruments give no indication of this distribution. However, in converting the micrometres reading to millitex units (Annex A1), low, medium, and high standard deviations were used in the calculations to arrive at the range of millitex units which accordingly reflect the distribution of fiber diameters.
|1) Balance Adjustment Knob||8) Porosity Calibration Control|
|2) Balance Pan||9) Compression Lever|
|3) Air Reservoir||10) Calibrator Plug Plunger|
|4) Meter Zero Adjustment Screw||11) Porosity Calibrator Plug|
|5) Porosity Test Chamber Lid||12) Calibration Weight|
|6) Differential Pressure Gage||13) Weighing Balance Mechanism|
|7) Porosity Zero Control||14) Atomizer Bulb|
|1) Metal specimen container||6) Gage tube|
|2) Packing rod||7) Millimetre scale|
|3) Plunger||8) Vacuum supply|
|4) Retaining collar||9) Upper gage tube mark|
|5) Control knob||10) Lower gage tube mark|
1.1 This test method covers the estimation of the average fiber diameter of wool fibers by use of the Port-Ar and the WIRA Fiber Fineness Meter instrument, which operate on the air-flow principle. Other air-flow instruments have not been tested with this method. The method is directly applicable to non-medullated, carded wool and wool top.
1.2 This test method is applicable to grease wool and scoured wool after the samples of such materials have been prepared as directed in Test Method D 2130 Note 1—The use of the Micronaire instrument for measuring the fineness of cotton fibers is covered in Test Method D 1448
The assignment of grade for wool and mohair is covered in Specifications D 3991
Note 1—The use of the Micronaire instrument for measuring the fineness of cotton fibers is covered in Test Method D 1448
1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D123 Terminology Relating to Textiles
D1060 Practice for Core Sampling of Raw Wool in Packages for Determination of Percentage of Clean Wool Fiber Present
D1448 Test Method for Micronaire Reading of Cotton Fibers
D2130 Test Method for Diameter of Wool and Other Animal Fibers by Microprojection
D3991 Specifications for Fineness of Wool or Mohair and Assignment of Grade
D3992 Specifications for Fineness of Wool Top or Mohair Top and Assignment of Grade
D4845 Terminology Relating to Wool
Other StandardIWTO-28-82(E) Determination By The Airflow Method of the Mean Fibre Diameter of Core Samples of Raw Wool
ICS Number Code 59.060.10 (Natural fibres)
UNSPSC Code 11151508(Wool fibers)
ASTM D1282-05(2009), Standard Test Method for Resistance to Airflow as an Indication of Average Fiber Diameter of Wool Top, Card Sliver, and Scoured Wool, ASTM International, West Conshohocken, PA, 2009, www.astm.orgBack to Top